Contents lists available atScienceDirect
Results in Physics
Area-selective electrodeposition of micro islands for CuInSe
, Daniel Siopab,1
, Diego Colombaraa
, Sara Tombolatob
, Pedro M.P. Saloméa
, Pedro Anacletoa
, Phillip J. Daleb
, Sascha Sadewassera,⁎
aInternational Iberian Nanotechnology Laboratory (INL), 4715-330 Braga, Portugal
bPhysics and Materials Science Research Unit, University of Luxembourg, L-4422 Belvaux, Luxembourg
A R T I C L E I N F O Keywords: Electrodeposition Ultra-micro electrodes Cu(In,Ga)Se2 Solar cells A B S T R A C T
For mass fabrication of highly-eﬃcient photovoltaic modules based on Cu(In,Ga)Se2(CIGSe) absorber layers the
availability and cost of the critical raw materials In and Ga present a potential bottleneck. The micro-con-centrator solar cell concept provides a solution by using micro lenses to concentrate incoming sun light on an array of micro-sized CIGSe solar cells. The challenge is to fabricate CIGSe micro islands in exactly the desired positions using only the required material. Here, we analyze the area-selective electrodeposition of CuInSe2into
holes in an insulating SiO2template layer as a material-eﬃcient fabrication approach. We observe that the
deposition process shows a strong dependence on the hole size, with a faster deposition around the hole peri-meter. Based on a model developed for electrochemical reactions at ultra-micro electrodes, we develop nu-merical simulations for the electrochemical deposition process. The simulations consider the changing micro-electrode geometry throughout the deposition process, and provide a reasonableﬁt to the experimental data. Finally, it is shown that CuInSe2micro solar cells fabricated by electrodeposition reach eﬃciencies of 4.8%
under 1 sun, providing a proof-of-concept demonstration meriting further development.
Cu(In,Ga)Se2(CIGSe) solar cells reach the highest power conversion
eﬃciency of all thin-ﬁlm photovoltaic technologies, with the present record at 22.9%[1,2]. The CIGSe absorber layer in highly eﬃcient cells is deposited under vacuum, either by co-evaporation from elemental precursors or by sputtering and subsequent reaction in selenium and/or sulfur atmosphere. However, the availability and cost of In and Ga have been raised as a concern for large-scale fabrication and installation of CIGSe PV. The micro-concentrator solar cell concept [5,6]has been proposed as a way to reduce the amount of In and Ga in CIGSe devices. The strategy is to use ordered micro lenses to con-centrate the impinging sunlight on a regular array of micrometer-sized CIGSe solar cells. For example, considering a perfect collection of all the impinging sunlight concentrated by a factor of 100 onto micro solar cells, this concept promises to reduce the amount of the critical raw materials In and Ga by the same factor, which is a considerable mate-rials savings. Proof-of-concept devices have been prepared by litho-graphically deﬁning micro cells from evaporated CIGSe material and have shown eﬃciencies of up to 21.3% under 475x. More recently,
proof-of-concept line-shaped and micro-island CIGSe devices have demonstrated the full materials-saving potential of the concept, leading to eﬃciencies of ∼5% and ∼0.3%, respectively. In both cases, the micrometer-sized absorbers were realized by selective area elec-trodeposition on conﬁned Mo electrodes.
For large area electrodes, the current (IC) of an electrochemical
process in solution depends essentially on the bulk concentration of the species j involved (Cj0), its diﬀusion coeﬃcient (Dj), and the number of electrons (n) transferred in the process, as described by Cottrell:
= I n F A C D πt C j0 j (1) where t is the deposition time, F the Faraday constant, and A the area of deposition. The Cottrell equation applies for the deposition after a voltage change between the electrodes and for situations where the supply of the depositing species is limited by their diﬀusion in solution. When using a rotating disk electrode (RDE), the supply of species can be faster and the deposition follows the Levich equation:
IL 0.62n F A D2/3ω1/2 v 1/6C (2)
Received 14 February 2019; Accepted 15 February 2019
E-mail address:Sascha.Sadewasser@inl.int(S. Sadewasser).
1These authors contributed equally to this work.
Available online 20 February 2019
2211-3797/ © 2019 The Authors. Published by Elsevier B.V. This is an open access article under the CC BY-NC-ND license (http://creativecommons.org/licenses/BY-NC-ND/4.0/).
whereω is the angular rotation rate of the electrode and v is the ki-nematic viscosity.
However, local electrochemical processes require special con-sideration of the geometry for their correct description, such as the case here, electrodepositing into arrays of micro-disk shaped electrodes. For the case of spatially conﬁned electrochemical reactions, in the 1980s Wightmanand Fleischmannintroduced the concept of ultra-micro electrodes (UME), which are generally considered to be∼20 µm or smaller. In this case, the species can only react in speciﬁc, locally conﬁned areas and diﬀusion occurs also laterally, from areas where no reaction can occur to those where the reaction takes place. The overall reaction rate then depends on the number N of disk-shaped UMEs, for which the total electrochemical current is[13,14]:
IUME i N 4r n F D C N (3)
where r is the radius of the micro electrodes. Eq.(3)applies for aﬂat electrode design. For the case of recessed UMEs, a correction factor considering the depth of the electrode has to be included and the cur-rent becomes: = = ⎛ ⎝ + ⎞⎠ − I i N r n F D C N π r L π r 4 4 UME r (4) where L is the depth of the electrode.
In this work, we investigate the deposition of CuInSe2 into
holes created in a SiO2insulating coating on top of a conductive
sub-strate. We show that the deposition depends strongly on the hole size. Therefore, we extend the equation describing electrochemical reactions at UMEs to the case of electrodeposition. Finally, we show completed proof-of-concept CIGSe micro solar cell devices obtained by electro-deposition in 200 µm-sized holes in SiO2.
To realize an area-selective electrodeposition process, we fabricated a patterned substrate allowing exposure to the deposition solution only in desired locations of the electrode surface. These pre-structured
substrates consist of a soda lime glass sheet (1 mm thickness) with a Mo metallic contact (500 nm thickness deposited by sputtering). A 2 µm thick SiO2layer is deposited by plasma-enhanced chemical vapor
de-position. Photolithography using a direct write laser is used to pattern a resist, followed by a reactive ion etching to etch the SiO2layer down to
the Mo contact. The remaining resist is removed using plasma ashing, followed by rinsing with acetone. Details about the fabrication process can be found in Ref.. For the present study, we fabricated a series of holes with diameters ranging from 4 µm to 500 µm.
The electrodeposition of CuInSe2is realized potentiostatically using
a three-electrode cell setup with a saturated calomel reference electrode (SCE). The counter electrode is a 3 × 3 cm2Pt mesh and the working
electrode is the pre-structured substrate with the series of holes. For all depositions a potential of−0.55 V vs. SCE was applied and the solution was stirred at 60 rpm. The sulfate-based solution contained 2 mM CuSO4, 3.89 mM In2(SO4)3, 4.0 mM SeO2, and 0.26 M Li2SO4as
sup-porting electrolyte. The CuInSe2micro islands were subsequently
selenized for 15 min at 500 °C in a tube furnace; a Se atmosphere was ensured by providing elemental Se as a precursor powder.
For the preparation of micro solar cell devices, the sequential electrodeposition process was chosen to allow the additional in-corporation of Ga in the future. To avoid any inﬂuence of diﬀerently-sized holes, substrates with arrays of identical holes were prepared according to the above described procedure. Initially, Cu was deposited into the holes using a rotating disk electrode (RDE) and a basic Cu solution containing 3.0 M NaOH, 0.2 mM sorbitol, and 0.1 M CuSO4. A
deposition voltage of−1.15 V vs. a Ag/AgCl reference electrode was used. Subsequently, In and Ga were deposited simultaneously in an In-Ga electrolyte with 50 mM InCl3and 25 mM GaCl3in reline mixture of
choline chloride and urea. The deposition was performed at 60 °C inside a N2-ﬁlled glovebox. Details about the electrodeposition can be found in
Ref.. To convert the Cu-In-Ga metallic precursor stack into CIGSe, the samples were pre-annealed for 30 min at 100 °C, followed by a se-lenization step of 20 min at 450 °C using an elemental Se source. To ensure good electrical performance, a KCN etch was performed to re-move any residual Cu2-xSe phases. Complete solar cell devices were
Fig. 1. Electrodeposition of CuInSe2into holes of (a) 12 µm, (b) 100 µm, and (c) 500 µm diameter in a SiO2matrix. For each diameter, an optical microscopy image is
shown as the background and proﬁlometer measurements show the thickness of the deposited CuInSe2for two scan lines (forward– solid line, backward - dashed
line). The blue circle indicates the original hole in the SiO2matrix. (d) Overview SEM image of a 100 µm hole with the CuInSe2deposit and (e) high-magniﬁcation
image of the typical morphology of electrodeposited CuInSe2. (f) Micro-Raman spectroscopy of the CuInSe2deposited inside a hole, clearly showing the typical A1
then fabricated by a standard CdS chemical bath deposition (50–70 nm thickness) and sputtering of a 90 nm thick i-ZnO and a 350 nm thick ZnO:Al layer.
Deposition of CuInSe2micro islands
The simultaneous deposition of Cu, In, and Se was realized on substrates containing a series of micro electrodes with diameters ran-ging from 4 µm to 500 µm. The micro electrodes consist of a Mo elec-trode at the bottom of a hole in a SiO2insulating layer of 2 µm
thick-ness. Fig. 1(a)–(c) show exemplary results of the electrodeposition process for holes with diameter of 12 µm, 100 µm, and 500 µm, re-spectively. The optical microscopy images show clearly that the de-position only occurs at the de-position of the electrodes and not on the SiO2 matrix, according to expectation. This was independently
con-ﬁrmed by scanning electron microscopy (SEM) imaging (Fig. 1(d)). The typical microstructure of the CuInSe2electrodeposited material can be
observed in the close-up SEM image inFig. 1(e). Energy dispersive x-ray spectroscopy experiments of the electrodeposited material in the holes conﬁrm the CuInSe2 composition and Raman measurements show
clearly the A1 vibrational mode at 172 cm−1of the tetragonal CuInSe2
(Fig. 1(f)). However, irregular edges of the deposited material are observed, indicating some deposition around the circumference of the holes. The thickness of the deposited CuInSe2material was measured by
proﬁlometry and the respective curves are overlayed on the optical images in Fig. 1(a)–(c). For the smallest sizes, the holes are ﬁlled homogeneously and the material has grown out of the hole, see Fig. 1(a). For the larger holes,Fig. 1(b) and (c), we observe a thicker deposit at the perimeter of the holes, while at the center the CuInSe2
material does not reach the thickness of the SiO2layer (i.e. 2 µm). The
formation of this corona around the perimeter of the holes shows no dependence on the diameter of the hole and an average width of (15.3 ± 5.5) µm is found. The proﬁlometer data is used to extract the thickness of the CuInSe2layer and the height of the corona; both values
are plotted as a function of the hole diameter inFig. 2(a). While the corona height is independent of the hole size, the thickness of the CuInSe2deposit at the center of the holes shows a clear decrease for
holes with a diameter larger than 60 µm. These results clearly demon-strate the enhanced deposition in smaller holes.
To analyze the obtained results in more detail, we evaluate the Cottrell and Levich equations for the present deposition conditions. The thickness d of the deposited layer can be estimated according to:
= d I M t
F n ρ A (5)
where M is the molar mass of the deposited species (336.3 g/mol for CuInSe2), t is the deposition time,ρ the density of the material (5.7 g/
2), and A the area of deposition. The compound
elec-trodeposition was assumed to be self-limited by the diﬀusion of the slowest species (Cu, D = 6.5·10−6cm2/s). Using the currents I
from Eqs.(1) and (2), it is clear that a dependence on the hole size cannot be described by these equations. The two deposition regimes give a constant thickness independent of the area, illustrated by the horizontal dashed lines inFig. 2(a).
As described above, electrochemical processes at micro electrodes require the use of Eq.(3). The dependence of the deposition thickness for planar (dotted red line) and recessed (depth L = 2 µm, dashed line) micro electrodes on the electrode diameter are also illustrated. While these dependencies apply for electrochemical processes, in the present case it has to be considered that the electrode shape and size change with time as more and more material is being deposited. We therefore performed numerical simulations of the thickness of the deposited material, the results of which are shown by the solid red lines in Fig. 2(a) and (b). Initially, it is considered that the depth L of the re-cessed electrode decreases with deposition time. The dependence of the correction factor (see Eq.(4)) for recessed electrodes as a function of electrode diameter and recess depth L is illustrated inFig. 2(c). Once the hole isﬁlled, the material grows on top of the surface, which we approximate by a hemispherical shape where the thickness and the radius of the electrode change.Fig. 2(b) shows the time dependence of the thickness for three diﬀerent diameters where the numerical simu-lation for aﬁxed recess depth of 2 µm (dashed lines) is compared to our simulation for a deposition process with a variable electrode size and shape (solid lines). The thickness of the dot after a 20-minute deposition is extracted from these numerical simulations as a function of the initial electrode diameter, resulting in the solid line ofFig. 2(a).
Our numerical simulation of the deposition process for micro elec-trodes gives a better qualitative description of the size dependence, compared to the analytical solution for electrochemical processes ac-cording to Eqs.(3) and (4)and illustrated schematically inFig. 3(a) and
Fig. 2. Electrodeposition in micro-sized holes. (a) Experimental thickness of CuInSe2at the center of the deposit (solid circles) and the height of the corona (open
circles) as a function of microelectrode hole diameter (20 min electrodeposition at 60 rpm). For comparison, the thickness evolution is given for the case of an electrochemical process on a planar electrode (Eq.(3), dotted line), a recessed electrode (Eq.(4), dashed line), and for an actual electrodeposition considering material growth and the changing micro electrode shape and size, according to the numerical simulation shown in (b) (solid line). For comparison, also the Levich (60 rpm) and Cottrell limits are indicated (dotted horizontal lines). (b) Simulated growths of CuInSe2deposits on micro electrodes of selected sizes, for aﬁxed recess
(b). However, a quantitative agreement is not reached. We attribute the discrepancies to two major reasons. (i) The deposited material in our study is CuInSe2, which is a semiconductor; thus, the growth of theﬁlm
is accompanied by a voltage drop across the thickness of the electrode, which continuously shifts the eﬀective electrochemical potential to more positive values during plating. (ii) The size range of the electrodes in our study goes beyond the range which is typically considered a micro electrode. In fact, our experimental results for diameters up to 60 µm follow the schematic illustration in Fig. 3(c) and (d), corre-sponding to what would be expected for a typical micro electrode. Unlike in the Cottrell regime, additional reaction species diﬀuse from
regions outside the electrode, leading to higher currents and– in the case of electrodeposition– thicker deposited material. If the diameter of the electrode becomes larger, the diﬀusion of these species does not cover the full electrode anymore and enhanced deposition only occurs at the outer ring of the electrode. This enhanced deposition leads to the corona eﬀect observed in our study, which is schematically illustrated inFig. 3(e) and (f). The width of the corona should be related to the diﬀusion coeﬃcient of the depositing species, independent of the electrode size, in agreement with our experimental observation.
Cu(In,Ga)Se2micro solar cells
For the fabrication of micro solar cells, we used the sequential de-position of Cu and In, followed by a high–temperature anneal in Se atmosphere to convert the Cu-In precursor into CuInSe2. To test the
suitability of the above described electrodeposition process, the de-position of the metallic precursor was performed into the same SiO2
matrices with holes. An array of 13 × 13 CuInSe2micro absorbers with
a diameter of 200 µm was then processed to full solar cell devices by deposition of CdS and the i-ZnO/ZnO:Al window layers. Subsequently, a single cell was isolated by scratching carefully the window layer stack on top of the SiO2matrix around the selected device (Fig. 4(a)). For the
measurement of the current density (J)-voltage (V) characteristics, four contacts were placed, two of them on the Mo back contact and the other two directly on the ZnO:Al layer on the SiO2insulating layer close to
the selected device. The JV characteristics presented inFig. 4(b) show a well performing solar cell with an open-circuit voltage of Voc= 396 mV, a short-circuit current of Jsc= 25.2 mA/cm2, and aﬁll
factor of FF = 48%, leading to a power conversion eﬃciency of 4.8%. These device results clearly show the suitability of the approach to electrodeposit CuInSe2into holes in an insulating matrix to realize the
materials-eﬃcient fabrication of micro-concentrator solar cells. Optimization of the electrodeposition process is required to address the above-described geometry-dependent deposition results.
We have presented a detailed analysis of the electrodeposition process into recessed micro electrodes by extending the analytical equations for electrochemical reactions in microelectrodes using nu-merical simulations to account for the size and shape change of the electrodes throughout the deposition process. Our results provide a qualitative description of the electrodeposition of CuInSe2into recessed
micro electrodes, which are studied for their application in photovoltaic energy conversion implementing the micro-concentrator thinﬁlm solar cell concept. To demonstrate this novel PV concept, CuInSe2micro solar
cells of 200 µm diameter were fabricated and their eﬃciency was measured to be 4.8% under 1 sun. Our study provides valuable insights into microelectrode electroplating, which is also relevant for many
Fig. 3. Schematic illustration of deposition geometry and the diﬀusion of spe-cies in solution for chemical reaction processes above (a) a micro electrode and (b) a recessed micro electrode. For an electrodeposition process, the material being deposited causes changes to the shape and size of the micro electrode during the deposition: (c) A small recessed microelectrodeﬁlls up, reducing the recess depth L and eventually (d) the material grows in a hemispherical way out of the micro electrode. For larger micro electrodes, the additional species that arrive from areas where no deposition occurs will lead to a corona eﬀect in-creasing the thickness of deposited material (e) inside the recessed micro electrode and (f) leading to thicker deposit (hc) at the circumference of the
initially recessed microelectrode.
Fig. 4. (a) Optical microscope image of a 6 × 2 sub-array of 200 µm-diameter CuInSe2micro solar cells
other applications from sensing to microfabrication. For the presented micro solar cells, we demonstrated proof-of-concept devices paving the way for further developments of this promising PV concept.
This work was partially supported by the project Nanotechnology Based Functional Solutions (NORTE-01-0145-FEDER-000019), sup-ported by Norte Portugal Regional Operational Programme (NORTE2020), under the PORTUGAL 2020 Partnership Agreement, through the European Regional Development Fund (ERDF). We ac-knowledge additional support by the Micro-concentrator thinﬁlm solar cells project (028922), co-funded by FCT and the ERDF through COMPETE2020. Funding by the Luxemburgish Fond National de la Recherche (FNR) through the MASSENA project is gratefully acknowl-edged. K.A. would like to acknowledge the Marie-Curie-COFUND pro-gram NanoTRAINForGrowth (grant agreement N°600375). DC thanks INL and the European Commission for funding the Nano Train for Growth II project n. 713640 through the Marie Curie Cofund pro-gramme.
The raw/processed data required to reproduce theseﬁndings cannot be shared at this time as the data also forms part of an ongoing study.
 Green MA, Emery K, Hishikawa Y, Warta W, Dunlop ED, Levi DH, et al. Solar cell eﬃciency tables (version 49). Prog Photovoltaics: Res Appl 2017;25:3–13.  Solar Frontier press release, 20.12.2017,http://www.solar-frontier.com/eng/news/
 Jackson P, Wuerz R, Hariskos D, Lotter E, Witte W, Powalla M. Eﬀects of heavy alkali elements in Cu(In, Ga)Se2solar cells with eﬃciencies up to 22.6%. Phys
Status Solidi RRL 2016;10:583–6.
 Wadia C, Alivisatos AP, Kammen DM. Environ Sci Technol 2009;43:2072.  Paire M, Lombez L, Donsanti F, Jubault M, Collin S, Pelouard J-L, et al. Thin-ﬁlm
microcells: a new generation of photovoltaic devices. SPIE Newsroom 2013.https:// doi.org/10.1117/2.1201305.004808.
 Paire M, Lombez L, Donsanti F, Jubault M, Collin S, Pelouard J-L, et al. Cu(In, Ga) Se2microcells: high eﬃciency and low material consumption. J Renew Sustain
 Duchatelet A, Nguyen K, Grand P-P, Lincot D, Paire M. Self-aligned growth of thin ﬁlm Cu(In, Ga)Se2solar cells on various micropatterns. Appl Phys Lett
 Sadewasser S, Salomé P, Rodriguez-Alvarez H. Materials eﬃcient deposition and heat management of CuInSe2micro-concentrator solar cells. Sol Energy Mater Sol
 Cottrell FG. Der Reststrom bei galvanischer Polarisation, betrachtet als ein Diﬀusionsproblem. Z Phys Chem 1903;42U:385–431.
 Levich VG. Physicochemical Hydrodynamics. Prentice-Hall; 1962.
 Wightman RM. Microvoltammetric electrodes. Anal Chem 1981;53:1125A–34A.  Fleischmann M, Pons S, Rolison DR, Schmidt PP. Ultramicroelectrodes. Morganton,
NC: Datatech Systems Inc; 1987.
 Bard AJ, Faulkner LR. Electrochemical methods: fundamentals and applications. John Wiley & Sons; 2001.
 Stulík K, Amatore Ch, Holub K, Marecek V, Kutner W. Microelectrodes. Deﬁnitions, characterization, and applications (Technical report). Pure Appl Chem
 Chassaing E, Grand P-P, Ramdani O, Vigneron J, Etcheberry A, Lincot D. Electrocrystallization mechanism of Cu–In–Se compounds for solar cell applica-tions. J Electrochem Soc 2010;157(7):D387–95.
 Sene C, Calixto ME, Dobson KD, Birkmire RW. Electrodeposition of CuInSe2
ab-sorber layers from pH buﬀered and non-buﬀered sulfate-based solutions. Thin Solid Films 2008;516:2188–94.
 Malaquias JC, Regesch D, Dale PJ, Steichen M. Simultaneous electrodeposition of indium and gallium from a choline chloride based deep eutectic solvent for Cu(In, Ga)Se2solar cells. PCCP 2014;16:2561–7.
 Aida Y, Depredurand V, Larsen JK, Arai H, Tanaka D, Kurihara M, et al. CuInSe2
solar cells with a Cu-poor surface. Prog Photovoltaics: Res Appl 2015;23:754–64.  Rincon C, Ramirez FJ. Lattice vibrations of CuInSe2and CuGaSe2by Raman